Abstract
Magnetic interactions in topological insulators cause essential modifications in the originally massless surface states. They offer a mass gap at the Dirac point and/or largely deform the energy dispersion, providing a new path towards exotic physics and applications to realize dissipationless electronics. The nonequilibrium electron dynamics at these modified Dirac states unveil additional functions, such as highly efficient photon to spincurrent conversion. Here we demonstrate the generation of large zerobias photocurrent in magnetic topological insulator thin films on midinfrared photoexcitation, pointing to the controllable band asymmetry in the momentum space. The photocurrent spectra with a maximal response to the intraDiracband excitations can be a sensitive measure for the correlation between Dirac electrons and magnetic moments.
Similar content being viewed by others
Introduction
Bismuthchalcogenidesbased topological insulators^{1} (TIs) generally have the bulk band gap of several hundreds meV, where the conduction and valence bands are connected by the surface states: massless Dirac dispersions with spinmomentum locking. When doped with magnetic elements^{2}, a Diracmass gap opens and/or the energy dispersion deforms (Fig. 1a) through the breaking of timereversal symmetry^{3,4,5}. The toplogical character of the surface states survives up to a moderate doping density, and offer a fertile ground of quantum phenomena, for example, creation of magnetic monopoles^{6}, quantized magnetoelectric effects^{7,8,9,10,11,12} and quantum anomalous Hall effects^{13,14,15}.
The corresponding Hamiltonian can be expressed as^{16}
where each term represents particlehole asymmetry (k is momentum, and m* the effective mass), spinorbit interaction resulting in the helical spin state (v_{k} is velocity and σ the Pauli matrices), hexagonal warping with amplitude λ (k_{±}≡k_{x}±ik_{y}), and coupling of electron’s spin to localized dopant spin S (n is the density and J is the interaction energy), respectively^{5,16,17}, with the unit of ħ=1. Here we take Cartesian coordinates with z along the surface normal. For the outofplane alignment of the dopant moments, either by magnetic anisotropy or by external fields, the spins turn parallel to z near the gapped Dirac point in the energy spectrum, and the Diracmass gap scales with JnS_{z}. This dispersion shows 3fold symmetry around the k_{z} axis^{5}, leading to an isotropic optical response in the linear regime. The Diracmass gap 2Δ of 60 meV was experimentally confirmed recently on a local scale in the case of Crdoped (Bi,Sb)_{2}Te_{3} ferromagnetic TIs^{18}. For the case of inplane magnetization, for example, the finite S_{y}, the gap closes or substantially reduces, with the Dirac point shifted from the zone center along k_{x} due to the Zeeman effect (Fig. 1a). Accordingly, the constant energy contour deforms by leaving one mirror plane in the momentum space^{5}. This asymmetry can induce transient spin and charge currents on photoexcitation^{19}.
In addition to intensive optical spectroscopy^{20,21,22,23,24,25,26,27}, a number of photoeffects in TIs have been studied both theoretically and experimentally; photocurrent generation and galvanic effects^{28,29,30,31,32}, carrier/spin dynamics elaborated by timeresolved optics^{33,34,35,36,37,38,39,40,41}, photoemission^{42,43,44,45,46,47,48,49,50,51} and the Floquet state^{52}, including the cases of thin films with magnetic dopants^{53,54}, to name a few. For the photocurrent generation at the normal incidence, it is predicted that the orbital coupling of light, that is, ħ→ħ−e, provides a predominant contribution to the polarizationindependent photocurrent under an inplane external magnetic field^{17}.
In this paper, we study photocurrent spectra in Cr_{0.3}(Bi_{0.22}Sb_{0.78})_{1.7}Te_{3} (CBST) thin films with a thickness of 8 nm. These samples are designed to achieve the following properties: The Fermi level is tuned near the Dirac point, which is isolated from the bulk states^{18,55}. The top and bottom surfaces hosting Dirac states are decoupled with the minimal contribution of the bulk volume in between. The dopant concentration is increased from those of the previous works^{13,14,15} to enhance magnetic transition temperature, T_{C}. Thus, intrinsic signals from the Dirac electrons^{49} interacting with magnetic dopants can be explored at moderate temperature. We show the generation of large zerobias photocurrent on midinfrared photoexcitation at normal incidence (Fig. 1b), realized by the fieldcontrollable band asymmetry in the momentum space. The enhanced response at the intraDiracband excitation would reveal intrinsic interactions between Dirac electrons and magnetic moments.
Results
Transport properties
Figure 1c shows that the fabricated CBST film is nonmetallic at room temperature, and the conduction through the surface states becomes apparent slightly below the T_{C}∼75 K, due to the freezing of thermally excited carriers in the bulk state and also reduced magnetic impurity scatterings^{14} (Supplementary Fig. 1). The Hall resistivity data (Fig. 1d) also illustrate the T_{C} and clear magnetic hysteresis loops at lower temperatures. In fact, the thinfilm sample, prepared at the similar growth condition but with smaller Cr concentration, was proven to show the quantum anomalous Hall effect as the hallmark of the above features of our sample design^{14}.
Zerobias photocurrent spectra
Figure 2a,b show the representative zerobias photocurrent under the inplane (B_{y}) and outofplane (B_{z}) external magnetic fields measured at 20 K, compared with the sample magnetization (ΔM, after subtracting the substrate contributions). Only in the case of applying B_{y}, a large photocurrent was detected. The current is nearly proportional to the inplane magnetization; it reverses when the magneticfield direction (or spin S_{y}) is flipped. A slight asymmetry at the positive and negative fields could be ascribed to the nonequivalent electrodes geometry. The photocurrent spectra show a pronounced peak around 250 meV (Fig. 2c). These characteristics were found to be independent of the incident photon polarization^{17}. The bulk band gap is anticipated to be around 300 meV, therefore the lowenergy photoresponses, at least <300 meV, can be ascribed to the dynamics of the spinpolarized Dirac electron at the surface. There exist some fluctuations in the photocurrent spectra, such as the increase of photocurrent around 100 meV under 0 T, whose origins are not clear at this stage.
Temperature and magneticfield dependence
Detailed characteristics of the zerobias photocurrent are shown in Fig. 3. The inflection behaviour in the magneticfield dependence diminishes around 80 K (Fig. 3a), consistent with the trend of inplane magnetization (Fig. 3b) and the Hall resistance data (Fig. 1d). The temperature dependence of the photocurrent nicely follows that of the magnetization (Fig. 3c).
Discussion
For the case of normal incidence in general, an imbalance in the electron excitation at the opposite k, and nonequilibrium carrier distributions on relaxation, can trigger the generation of directional photocurrent^{19}. This photocurrent can be enhanced by the spinorbit interaction, most prototypically for the surface Dirac electrons with the deformed Dirac dispersions as in the present case. In our experiments, possible contributions from the photogalvanic effect due to the trigonal warping can be neglected, judging from the absence of photocurrent at zero field. Neither the NernstEttingshausen effect nor the photon drags have roles in our optical geometry.
The observed zerobias photocurrent in the magnetic TI thin film can be explained by the magnetizationinduced modification of the energy dispersion (Fig. 4), making both the excitation and relaxation at ±k asymmetric. In the absence of external fields, or under the application of B_{z}, the doped Cr moment induces the Diracmass gap. In this case, the constant energy contour of the dispersion remains symmetric in the k_{x}k_{y} plane (Fig. 4a,d). In stark contrast, with the application of −B_{y} (induction of S_{y}), the Diracmass gap closes, and the energy contour shifts/deforms orthogonal to the orientation of magnetic moment (towards k_{x} for S_{y}) (Fig. 4b,e). Here we draw the energy contours in Fig. 4d,e, by following equation (1) with the parameters in refs 5, 19, and 2Δ=60 meV from ref. 18. These shifts and deformations are proportional to the inplane moment S_{y}, and the latter have a major role for the photocurrent generation.
When the photon energy is below 300 meV, within the bulk band gap where the observed photocurrent largely enhances, the photoexcitation between the bulk valence and conduction bands can be neglected. Given that the Fermi level is located near the Dirac point, we can expect two pathways of Dirac electronrelated excitation and relaxation; excitation within the surface states (Fig. 4b), and between the surface states and the bulk states (and vice versa) (Fig. 4c). We will exclude the latter process as the major mechanism of photocurrent generation in the following, since merely small photocurrent observed at the higher photon energy (Fig. 2c). The surface state as the final state of the optical excitation is important for the observed photocurrent, where the asymmetry in the dispersion is directly involved.
Now we discuss the spectral structure as exemplified by the peak around 250 meV (Fig. 2c). The optical processes possibly involved in the present photogalvanic effect have been discussed theoretically in refs 5, 19. In short, the zerobias photocurrent flows due to the unbalanced transient carrier population (f(k): FermiDirac function) in the deformed Dirac dispersions, that is, f(k_{x})−f(−k_{x}), multiplied by the group velocity, which can be proportional to the local magnetic moment. The optical absorption in the surface Dirac states is supposed to be nearly monotonic as a function of photon energy in our spectral range^{19,21,22,23,24,25,54} (see also Supplementary Fig. 2). However, the observed photocurrent shows a clear peak around 250 meV; it decreases towards zero in lowering photon energy and also shows a reduction in increasing photon energy above 250 meV. The former trend is predicted in ref. 19 as due to the decreased asymmetry near the Dirac point (compare the grey and orange transitions in Fig. 4b). Even with the finite optical absorption, the photocarriers with the opposite group velocity would cancel for the lowenergy excitation. The decrease in the photocurrent at higher energy can be ascribed to the pronounced scattering between bulk and surface states (Fig. 4c), which is not taken into account in ref. 19. Here the optical transition to the bulk states increases in the photon energy region above ∼250 meV, and most of the population asymmetry is lost above 500 meV due to the scattering between the bulk and surface states. Note that we have finite potential fluctuations in the film, including those of ∼20 meV from Cr dopants^{18} and also between the two surface states (see below), which can induce broadenings in the photocurrent spectra. The small but finite photocurrent under B_{z} (Fig. 2b) may point to the effect of hexagonal warping with the spin moments oriented along z, which is ignored in the above analyses^{5}.
Considering the thickness of our sample (8 nm), the top and the bottom surface states (the latter is the interface between CBST and InP) experience nearly the same optical fields for the lowphotonenergy region (Supplementary Fig. 2). In the abovediscussed model, the energy contour shifts/deforms in the opposite direction for the top and bottom surface states; the excited photocarriers flow in the counter direction, which may cancel at the end. However, in general, the top and bottom surface states are inevitably inequivalent^{9} due to their distinct environments and growth characteristics. The energy shift of the surfacestate electronic bands is estimated as large as 5070 meV from the quantum Hall effect measurements^{56}. Thus we detect the photocurrent portion not cancelled in the two surface states. By checking the signals from the sample with a modulated Cr doping, we found an indication that the bottom surface has the larger contribution to the photocurrent in the present case (Supplementary Fig. 3). It is also seen that we can possibly enhance the photocurrent by further differentiating the top and bottom surface states. However, a quantitative discussion is difficult at this stage because of the extrinsic factors such as the change in the transition temperature and scatterings by dopants.
The amplitude of the detected photocurrent, although transient, reaches a value as large as 60 μA cm^{−1} (Fig. 2a with the experimental geometry taken into account). This is more than two orders of magnitude larger than that observed by the circular photogalvanic effect in the bulk Bi_{2}Se_{3} (ref. 30), in which the obliqueincidence circularly polarized light can inject the spins in the Dirac dispersion to generate the zerobias current. This is also larger than the theoretically predicted values with magnetic proximity interactions^{19} (see also Supplementary Fig. 4). Considering the relaxation of photoexcited carriers before reaching the electrodes, the instantaneous photocurrent would be even much larger. In the experiments shown above, we used the external magnetic field larger than ∼0.5 T to orient the Cr moments (and to generate the photocurrent). If we could prepare the sample with an easyplane anisotropy, it would be possible to have a spinpolarized photocurrent in zero field, whose direction could be controlled by the switching of the magnetic domains. As such, the magnetic control of the nonequilibrium Dirac electrons in the magnetic topological insulator will pave a new path for intriguing spintronic functions.
Methods
Sample preparation and characterization
Thin films of CBST were grown on InP(111) substrates by the molecular beam epitaxy, where the similar films with the smaller Cr concentration have been proven to show the quantum anomalous Hall effect. The detailed growth conditions are described in ref. 14. The surface was protected by a 3 nm thick Al_{2}O_{3} cap layer. The samples were characterized by conventional transport and magnetization measurements. The diamagnetic contribution of the substrate was subtracted for the latter.
Photocurrent detection
Two AuPd electrodes were deposited along the [100] axis after removing the cap layer. The shortcircuit photocurrent was measured through a wideband preamplifier (bandwidth of 200 MHz) with the illumination by a pulsed laser source (120 fs, 1 kHz, spot size 1.0–0.5 mm in diameter) at normal incidence. The excitation spot was carefully positioned at the center of the sample to cancel possible thermoelectric signals (Supplementary Fig. 5). The time trace of the photocurrent was averaged 150 times in the digitizing oscilloscope, which was broadened by the response of the preamplifier and followed by ringing due to the impedance mismatch in the circuit (Fig. 2a). The magnetic field and photon energy dependencies were obtained by averaging more than 2,048 signal pulses after gating the photocurrent signal by a boxcar averager. The acquired signal was normalized by the integrated timetrace from the oscilloscope, as a number of charge, and also by the incident photon intensity. The error bars in our measurements are within the circle marks in Fig. 2c. We have checked three samples with slightly different compositions, and confirmed nearly the identical results.
Data availability
The data that support the findings of this study are available from the corresponding author on request.
Additional information
How to cite this article: Ogawa, N. et al. Zerobias photocurrent in ferromagnetic topological insulator. Nat. Commun. 7:12246 doi: 10.1038/ncomms12246 (2016).
References
Hasan, M. Z. & Kane, C. L. Topological insulators. Rev. Mod. Phys. 82, 3045–3067 (2010).
Li, M. et al. Experimental verification of the Van Vleck nature of longrange ferromagnetic order in the vanadiumdoped threedimensional topological insulator Sb2Te3 . Phys. Rev. Lett. 114, 146802 (2015).
Hor, Y. S. et al. Development of ferromagnetism in the doped topological insulator Bi2−xMnxTe3 . Phys. Rev. B 81, 195203 (2010).
Chen, Y. L. et al. Massive Dirac fermion on the surface of a magnetically doped topological insulator. Science 329, 659–662 (2010).
Henk, J. et al. Topological character and magnetism of the Dirac state in MnDoped Bi2Te3 . Phys. Rev. Lett. 109, 076801 (2012).
Qi, X.L., Li, R., Zhang, J. & Zhang, S.C. Inducing a magnetic monopole with topological surface states. Science 323, 1184–1187 (2009).
Qi, X.L., Hughes, T. L. & Zhang, S.C. Topological field theory of timereversal invariant insulators. Phys. Rev. B 78, 195424 (2008).
Tse, W.K. & MacDonald, A. H. Giant magnetooptical Kerr effect and universal Faraday effect in thinfilm topological insulators. Phys. Rev. Lett. 105, 057401 (2010).
Maciejko, J., Qi, X.L., Drew, H. D. & Zhang, S.C. Topological quantization in units of the fine structure constant. Phys. Rev. Lett. 105, 166803 (2010).
Li, R., Wang, J., Qi, X.L. & Zhang, S.C. Dynamical axion field in topological magnetic insulators. Nat. Phys 6, 284–288 (2010).
Valdés Aguilar, R. et al. Terahertz response and colossal Kerr rotation from the surface states of the topological insulator Bi2Se3 . Phys. Rev. Lett. 108, 087403 (2012).
Orlita, M. et al. Magnetooptics of massive Dirac fermions in bulk Bi2Se3 . Phys. Rev. Lett. 114, 186401 (2015).
Chang, C.Z. et al. Experimental observation of the quantum anomalous Hall effect in a magnetic topological insulator. Science 340, 167–170 (2013).
Chekelsky, J. G. et al. Trajectory of the anomalous Hall effect towards the quantized state in a ferromagnetic topological insulator. Nat. Phys 10, 731–736 (2014).
Chang, C.Z. et al. Highprecision realization of robust quantum anomalous Hall state in a hard ferromagnetic topological insulator. Nat. Mater. 14, 473–477 (2015).
Fu, L. Hexagonal warping effects in the surface states of the topological insulator Bi2Te3 . Phys. Rev. Lett. 103, 266801 (2009).
Junck, A., Refael, G. & von Oppen, F. Photocurrent response of topological insulator surface states. Phys. Rev. B 88, 075144 (2013).
Lee, I. et al. Imaging Diracmass disorder from magnetic dopant atoms in the ferromagnetic topological insulator Crx(Bi0.1Sb0.9)2−xTe3 . Proc. Natl Acad. Sci. 112, 1316–1321 (2015).
Semenov, Y. G., Li, X. & Kim, K. W. Tunable photogalvanic effect on topological insulator surfaces via proximity interactions. Phys. Rev. B 86, 201401 (R) (2012).
Chang, M.C. & Yang, M.F. Optical signature of topological insulators. Phys. Rev. B 80, 113304 (2009).
LaForge, A. D. et al. Optical characterization of Bi2Te3 in a magnetic field: infrared evidence for magnetoelectric coupling in a topological insulator material. Phys. Rev. B 81, 125120 (2010).
Di Pietro, P. et al. Optical conductivity of bismuthbased topological insulators. Phys. Rev. B 86, 045439 (2012).
Akrap, A. et al. Optical properties of Bi2Te2Se at ambient and high pressures. Phys. Rev. B 86, 235207 (2012).
Li, Z. & Carbotte, J. P. Hexagonal warping on optical conductivity of surface states in topological insulator Bi2Te3 . Phys. Rev. B 87, 155416 (2013).
Post, K. W. et al. Infrared probe of the bulk insulating response in Bi2−xSbxTe3−ySey topological insulator alloys. Phys. Rev. B 91, 165202 (2015).
Onishi, Y. et al. Ultrafast carrier relaxation through Auger recombination in the topological insulator Bi1.5Sb0.5Te1.7Se1.3 . Phys. Rev. B 91, 085306 (2015).
Wu, L. et al. Highresolution Faraday rotation and electronphonon coupling in surface states of the bulkinsulating topological insulator Cu0.02Bi2Se3 . Phys. Rev. Lett. 115, 217602 (2015).
Kastl, C. et al. Local photocurrent generation in thin films of the topological insulator Bi2Se3 . Appl. Phys. Lett. 101, 251110 (2012).
Bas, D. A. et al. Coherent control of injection currents in highquality films of Bi2Se3 . Appl. Phys. Lett. 106, 041109 (2015).
McIver, J. W., Hsieh, D., Steinberg, H., JarilloHerrero, P. & Gedik, N. Control over topological insulator photocurrents with light polarization. Nat. Nanotech. 7, 96–100 (2012).
Kastl, C., Karnetzky, C., Karl, H. & Holleitner, A. W. Ultrafast helicity control of surface currents in topological insulators with nearunity fidelity. Nat. Commun. 6, 6617 (2015).
Okada, K. N. et al. Enhanced photogalvanic current in topological insulators via Fermi energy tuning. Phys. Rev. B 93, 081403 (R) (2016).
Qi, J. et al. Ultrafast carrier and phonon dynamics in Bi2Se3 crystals. Appl. Phys. Lett. 97, 182102 (2010).
Hsieh, D. et al. Nonlinear optical probe of tunable surface electrons on a topological insulator. Phys. Rev. Lett. 106, 057401 (2011).
Kumar, N. et al. Spatially resolved femtosecond pumpprobe study of topological insulator Bi2Se3 . Phys. Rev. B 83, 235306 (2011).
Hsieh, D. et al. Selective probing of photoinduced charge and spin dynamics in the bulk and surface of a topological insulator. Phys. Rev. Lett. 107, 077401 (2011).
Sim, S. et al. Ultrafast terahertz dynamics of hot Diracelectron surface scattering in the topological insulator Bi2Se3 . Phys. Rev. B 89, 165137 (2014).
Glinka, Y. D., Babakiray, S., Johnson, T. A., Holcomb, M. B. & Lederman, D. Effect of carrier recombination on ultrafast carrier dynamics in thin films of the topological insulator Bi2Se3 . Appl. Phys. Lett. 105, 171905 (2014).
Boschini, F. et al. Coherent ultrafast spindynamics probed in three dimensional topological insulators. Sci. Rep. 5, 15304 (2015).
Maezawa, S. et al. Optically detecting the edgestate of a threedimensional topological insulator under ambient conditions by ultrafast infrared photoluminescence spectroscopy. Sci. Rep. 5, 16443 (2015).
Wang, M. C., Qiao, S., Jiang, Z., Juo, S. N. & Qi, J. Unraveling photoinduced spin dynamics in the topological insulator Bi2Sb3 . Phys. Rev. Lett. 116, 036601 (2016).
Sobota, J. A. et al. Ultrafast optical excitation of a persistent surfacestate population in the topological insulator Bi2Se3 . Phys. Rev. Lett. 108, 117403 (2012).
Sobota, J. A. et al. Direct optical coupling to an unoccupied Dirac surface state in the topological insulator Bi2Se3 . Phys. Rev. Lett. 111, 136802 (2013).
Cacho, C. et al. Momentumresolved spindynamics of bulk and surface excited states in the topological insulator Bi2Se3 . Phys. Rev. Lett. 114, 097401 (2014).
Hajlaoui, M. et al. Tuning a Schottky barrier in a photoexcited topological insulator with transient Dirac cone electronhole asymmetry. Nat. Commun. 5, 3003 (2014).
Reimann, J., Güdde, J., Kuroda, K., Chulkov, E. V. & Höfer, U. Spectroscopy and dynamics of unoccupied states of the topological insulators Sb2Te3 and Sb2Te2S. Phys. Rev. B 90, 081106 (R) (2014).
Shoman, T. et al. Topological proximity effect in a topological insulator hybrid. Nat. Commun. 6, 6547 (2015).
Xu, C.Z. et al. Photoemission circular dichroism and spin polarization of the topological surface states in ultrathin Bi2Te3 films. Phys. Rev. Lett. 115, 016801 (2015).
Neupane, M. et al. Gigantic surface lifetime of an intrinsic topological insulator. Phys. Rev. Lett. 115, 116801 (2015).
Kogar, A. et al. Surface collective modes in the topological insulators Bi2Se3 and Bi0.5Sb1.5Te3−xSex . Phys. Rev. Lett. 115, 257402 (2015).
Kuroda, K., Reimann, J., Gudde, J. & Hofer, U. Generation of transient photocurrents in the topological surface state of Sb2Te3 by direct optical excitation with midinfrared pulses. Phys. Rev. Lett. 116, 076801 (2016).
Wang, Y. H., Steinberg, H., JarilloHerrero, P. & Gedik, N. Observation of FloquetBloch states on the surface of a topological insulator. Science 342, 453–457 (2013).
Zhang, D. et al. Interplay between ferromagnetism, surface states, and quantum corrections in a magnetically doped topological insulator. Phys. Rev. B 86, 205127 (2012).
Lasia, M. & Brey, L. Optical properties of magnetically doped ultrathin topological insulator slabs. Phys. Rev. B 90, 075417 (2014).
Yoshimi, R. et al. Dirac electron states formed at the heterointerface between a topological insulator and a conventional semiconductor. Nat. Mater. 13, 253–257 (2014).
Yoshimi, R. et al. Quantumj Hall effect on top and bottom surface states of topological insulator (Bi1−xSbx)2Te3 films. Nat. Commun. 6, 6627 (2015).
Acknowledgements
We thank N. Nagaosa and W. Koshibae for stimulating discussions. This research is supported by JSPS KAKENHI Grant Numbers 24224009 and 16K13705.
Author information
Authors and Affiliations
Contributions
N.O., R.Y., A.T., M.K. and Y.T. conceived the experiment; R.Y., K.Y. prepared and characterized the samples; and N.O. carried out the optical experiments. N.O., R.Y., K.Y., A.T., M.K. and Y.T. wrote the manuscript. All authors contributed considerably.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing financial interests.
Supplementary information
Supplementary Information
Supplementary Figures 15 and Supplementary References (PDF 261 kb)
Rights and permissions
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
About this article
Cite this article
Ogawa, N., Yoshimi, R., Yasuda, K. et al. Zerobias photocurrent in ferromagnetic topological insulator. Nat Commun 7, 12246 (2016). https://doi.org/10.1038/ncomms12246
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/ncomms12246
This article is cited by

A candidate material EuSn2As2based terahertz direct detection and imaging
npj 2D Materials and Applications (2022)

Polarizationcontrolled tunable directional spindriven photocurrents in a magnetic metamaterial with threefold rotational symmetry
Nature Communications (2022)

Topology and geometry under the nonlinear electromagnetic spotlight
Nature Materials (2021)

Novel synthesis of topological insulator based nanostructures (Bi2Te3) demonstrating high performance photodetection
Scientific Reports (2019)

Magnetic topological insulators
Nature Reviews Physics (2019)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.